SUPERSEDED (click for Active standard)
| ||Format||Pages||Price|| |
|9||$52.80||  ADD TO CART|
1.1 This specification covers the requirements for electrodeposited cadmium coatings on products of iron, steel, and other metals.
Note 1—Cadmium is deposited as a coating principally on iron and steel products. It can also be electrodeposited on aluminum, brass, beryllium copper, copper, nickel, and powder metallurgy parts.
1.2 The coating is provided in various thicknesses up to and including 25 μm either as electrodeposited or with supplementary finishes.
1.3 Cadmium coatings are used for corrosion resistance and for corrosion prevention of the basis metal part. The as-deposited coating (Type I) is useful for the lowest cost protection in a mild or noncorrosive environment where early formation of white corrosion products is not detrimental or harmful to the function of a component. The prime purpose of the supplementary chromate finishes (Types II and III) on the electroplated cadmium is to increase corrosion resistance. Chromating will retard or prevent the formation of white corrosion products on surfaces exposed to various environmental conditions as well as delay the appearance of corrosion from the basis metal.
1.4 Cadmium plating is used to minimize bi-metallic corrosion between high-strength steel fasteners and aluminum in the aerospace industry. Undercutting of threads on fastener parts is not necessary as the cadmium coating has a low coefficient of friction that reduces the tightening torque required and allows repetitive dismantling.
1.5 Cadmium-coated parts can easily be soldered without the use of corrosive fluxes. Cadmium-coated steel parts have a lower electrical contact resistance than zinc-coated steel. The lubricity of cadmium plating is used on springs for doors and latches and for weaving machinery operating in high humidity. Corrosion products formed on cadmium are tightly adherent. Unlike zinc, cadmium does not build up voluminous corrosion products on the surface. This allows for proper functioning during corrosive exposure of moving parts, threaded assemblies, valves, and delicate mechanisms without jamming with debris.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
B183 Practice for Preparation of Low-Carbon Steel for Electroplating
B201 Practice for Testing Chromate Coatings on Zinc and Cadmium Surfaces
B242 Guide for Preparation of High-Carbon Steel for Electroplating
B253 Guide for Preparation of Aluminum Alloys for Electroplating
B281 Practice for Preparation of Copper and Copper-Base Alloys for Electroplating and Conversion Coatings
B320 Practice for Preparation of Iron Castings for Electroplating
B567 Test Method for Measurement of Coating Thickness by the Beta Backscatter Method
B568 Test Method for Measurement of Coating Thickness by X-Ray Spectrometry
B571 Practice for Qualitative Adhesion Testing of Metallic Coatings
B602 Test Method for Attribute Sampling of Metallic and Inorganic Coatings
B697 Guide for Selection of Sampling Plans for Inspection of Electrodeposited Metallic and Inorganic Coatings
E8 Test Methods for Tension Testing of Metallic Materials
F519 Test Method for Mechanical Hydrogen Embrittlement Evaluation of Plating/Coating Processes and Service Environments
Federal StandardQQ-P-416 Plating, Cadmium (Electrodeposited) Available from U.S. Government Printing Office, Washington DC 20402.
Military StandardMIL-STD-1312 Fasteners, Test Methods Available from Standardization Documents Order Desk, Bldg. 4 Section D, 700 Robbins Ave., Philadelphia, PA 19111-5094, Attn: NPODS.
ICS Number Code 25.220.40 (Metallic coatings)
ASTM B766-86(2003), Standard Specification for Electrodeposited Coatings of Cadmium, ASTM International, West Conshohocken, PA, 2003, www.astm.orgBack to Top